# A generalised Monkman-Grant relation for creep life prediction: An application to 1CrMoV rotor steel

Embed Size (px)

### Transcript of A generalised Monkman-Grant relation for creep life prediction: An application to 1CrMoV rotor steel

J M A T E R S C I 4 1 (2 0 0 6 ) 3 9 0 7 –3 9 1 5

A generalised Monkman-Grant relation for creep life

prediction: An application to 1CrMoV rotor steel

M. EVANSSchool of Engineering, University of Wales Swansea, Singleton Park, Swansea, SA2 8PP, UKE-mail: [email protected]

Published online: 12 April 2006

A generalised Monkman—Grant relation, which can be derived from the 4-� projectiontechnique, is proposed and then used to predict creep properties at non accelerated testconditions. In this generalisation, creep rates at low strains are used to predict minimum creeprates that are then used in the Monkman-Grant relation to predict times to failure. Predictions ofcreep properties for 1CrMoV from this generalisation and from the 4-� projection techniquewere assessed using the mean absolute percentage error (MAPE) and mean square error(MSE)—which was further decomposed into systematic and random components. Whenconsidering the accuracy with which minimum creep rates were predicted, all but thegeneralised Monkman-Grant relation using 0.1% strain had a lower MAPE compared to the4-�projection technique. The generalised Monkman-Grant relation using 0.5% and 1% strainshad larger random components of the MSE compared to the 4-�projection technique. Whenconsidering the accuracy with which times to failure were predicted, all of the generalisedMonkman-Grant relations produced lower MAPE compared to the 4-� projection technique.However, only when creep rates were measured at 0.2% strain, did the generalisedMonkman-Grant relation produce prediction errors that had a significantly higher randomcomponent. C© 2006 Springer Science + Business Media, Inc.

1. Introduction

Evans [1] has reviewed a number of creep property pre-diction models that have been used in the recent past. Themost successful of these include the 4-� and 6-θ pro-jection techniques developed and applied by Evans [2, 3]and Evans and Scharning [4], the continuum damage tech-niques (CDM) developed by Kachanov [5], Rabotnov [6]and latter generalised by Othman and Hayhurst [7] and the� methodology for the life assessment of components re-cently proposed by Prager [8]. What all these techniqueshave in common is the need to model the whole creepcurve using some specified non linear function in time.The parameters of this functional relationship then re-quire estimation using quite complicated non linear leastsquares procedures. This complication has limited the ex-tent to which these relatively successful techniques havebeen implemented and applied within industry.

When attempting to predict creep life, engineers facea variety of complex problems including stress triaxilityat stress inducing features, selection of hardening rules tobe applied for relaxing of cyclical loading and the selec-tion of suitable models for creep damage accumulation.Whilst these issues are undoubtedly important, this paper

concentrates on projection techniques suitable for analyz-ing the results from uniaxial constant stress tests.

In particular, the objectives of this paper are to firstdemonstrate that a simple but generalised Monkman-Grant type relation can be derived from the 4-� projectiontechnique which can be applied without the use of compli-cated non linear least squares techniques (which is centralto the 4-� projection technique). Then the predictive ca-pability of this generalised Monkman-Grant relation isassessed and compared to the 4-� projection techniqueusing a number of capability statistics not typically usedin the field of creep.

2. Experimental proceduresThe Interdisciplinary Research Centre at Swansea (IRC)carries out high temperature testing programs involvingmany different materials. The test matrices are such thatspecimens are tested at highly accelerated stress condi-tions, i.e. at stresses well in excess of the design stressfor such materials, but at close to operating temperatures.Further, all the tests are at constant stress and strain mea-surements are taken at regular time intervals so that de-tailed experimental creep curves are available.

0022-2461 C© 2006 Springer Science + Business Media, Inc.DOI: 10.1007/s10853-005-5506-7 3907

The batch of material tested at the IRC and used for thepresent investigation represents the lower bound creepstrength properties anticipated for 1CrMoV rotor steels.The chemical composition of this batch of material (inwt%) was determined as 0.27% C, 0.22% Si, 0.77% Mn,0.008% S, 0.015% P, 0.97% Cr, 0.76% Ni, 0.85% Mo,0.39% V, 0.125% Cu, 0.008% Al and 0.017% Sn. Follow-ing oil quenching from 1238 K and tempering at 973 K,the material had a tensile strength of 741 MPa (at roomtemperature), elongation of 17%, reduction in area of 55%and a 0.2% proof stress of 618 MPa.

Eighteen test pieces, with a gauge length of 25.4 mmand a diameter of 3.8 mm, were tested in tension over arange of stresses at 783, 823 and 863 K using high preci-sion constant-stress machines [9]. At 783 K, six specimenswere placed on test over the stress range 425 to 290 MPa,at 823 K seven specimens were placed on test over thestress range 335 to 230 MPa and at 863 K six specimenswere tested over the stress range 250 to 165 MPa. Upto 400 creep strain/time readings were taken during eachof these tests. Normal creep curves were observed underall these test conditions. Table Ia shows the times to fail-ure, minimum creep rates and creep rates at p (where pis in %) strain for all tested specimens. Creep rates weremeasured from the data points making up the experimen-tal creep curves using numerical derivates (i.e. a secondorder version of a lagrange interpolating polynomial).

To assess the extrapolative capability of these models,long-term property data was supplied independently by anindustrial consortium involving GEC-Alstom, BabcocksEnergy, National Power, PowerGen and Nuclear Electric.These longer-term properties came from the same batchof material used in the accelerated test programme de-scribed above but for specimens with gauge lengths of125 mm and diameters of 14 mm that were subjected totests on high sensitivity constant-load tensile creep ma-chines. Twelve specimens were tested in this way at 823 Kand at stresses ranging from 215 to 77 MPa.

This longer-term data was published by Wilshire et al.[10] and at the time of publication in 1993 the creep prop-erty measurements made on these 12 specimens wereincomplete. Table Ib summarises the full results of thislonger-term data set. As can be seen, at the very lowstresses only the times to low strains and creep rates atlow strains were recorded (as these specimens had notfailed when this data was published). Again creep rateswere measured from the strain-time measurements madeat p strain using numerical derivatives (i.e. a second or-der version of a lagrange interpolating polynomial). Un-like the short term data, all of these longer-term testswere carried out at constant load. The extent to whichvarious creep property values are affected by the choiceof constant load or constant stress methods depends onthe material ductility and the shape of the creep curve.As shown by Wilshire et al. [10], the minimum creeprates were virtually unaffected, whereas only small re-ductions in creep lives were observed for constant loadcondition.

The short-term data set is therefore made up of i = 1to N (where N = 18) specimens and the longer term dataset is made up of j = 1 to M (where M = 12) specimens.In what follows j and i will now be used to represent thetest condition at which the jth and ith specimens weretested. Predictions of minimum creep rates and times tofailure using the 4-� projection technique are taken fromEvans [11] and Table Ic presents some of these longer-term predictions.

3. Theoretical underpinnings of a generalisedMonkman-Grant relation

3.1. The 4-� projection techniqueThe 4-� projection technique starts of by measuring com-plete creep curves at a variety of different acceleratedtest conditions, i.e. for all test conditions making up theshort-term data set. Then each experimental creep curveis modeled using

εi,t = �i,1(1 − e−�i,2t ) + �i,3(e�i,4t − 1) (1a)

where εi,t is the strain at time t at accelerated test conditioni. The parameters �i,1 to �i,4 are estimated using quitecomplicated non linear least squares algorithms.

To predict the creep curve at or close to operating testconditions, these estimated theta parameters are then re-lated to the accelerated test conditions through the extrap-olation function given by

ln[�i,k] = βk,0+βk,1τi+βk,2Ti+βk,3τi Ti (1b)

where τ i is the stress at accelerated test condition i andTi is the temperature at the same test condition. With fourTheta parameters, k varies from 1 to 4. Values for the βk,l

parameters are estimated using complex weighted leastsquares procedures using only the accelerated test data.Weighting is required to deal with the fact that some ofthe Theta parameters are estimated with more reliabilitythan others—depending on the experimental scatter in themeasured creep curve.

Equation 1b is then used to predict the Theta valuesassociated with operating condition j, � j,k . These are thensubstituted into Equation 1a to predict the shape of thecreep curve at this operating condition. From this creepcurve a range of creep properties can be read off. Evans[2 ] explains in detail how minimum creep rates, times tofailure and times to various strains can be read off fromthe predicted creep curve.

A procedure not normally used in the theta projectiontechnique is to use the Monkman-Grant relation [12] toobtain a life time prediction

ln(t j, f ) = λ0 + λ1 ln(ε j,m) (2)

where values for λ0 and λ1 are estimated using linearleast squares from the accelerated test data only and ε j,m

is read off the predicted creep curve. Whilst doubt hasbeen expressed in the past by Dobes and Malicka [13 ] and

3908

T AB L E I A Results making up the shorter-term data set

Creep rate (h−1) at p strain

Temp. (K) Stress (MPa) 0.05% 0.1% 0.2% 0.5% 1% Failure time (h)Min. creep rate(h−1)

783 425 1.70E–2 1.45E–2 1.20E–2 6.88E–3 4.51E–3 14.06 4.18E–3783 370 1.18E–3 1.04E–3 8.72E–4 3.83E–4 2.91E–4 180.99 2.80E–4783 350 1.61E–3 1.30E–3 4.90E–4 1.82E–4 1.38E–4 218.28 1.37E–4783 320 5.94E–4 5.08E–4 2.44E–4 1.13E–4 8.81E–5 387.81 8.88E–5783 305 1.29E–4 1.10E–4 7.89E–5 3.16E–5 3.21E–5 1469.89 2.77E–5783 290 9.26E–5 5.43E–5 3.18E–5 1.41E–5 1.39E–5 4458.61 1.28E–5823 335 1.11E–2 9.41E–3 8.17E–3 3.88E–3 2.63E–3 30.55 2.55E–3823 310 6.35E–3 6.00E–3 3.92E–3 9.77E–4 7.18E–4 67.46 6.55E–4823 290 5.10E–3 4.53E–3 2.33E–3 1.05E–3 7.56E–4 68.00 7.74E–4823 270 6.24E–4 5.93E–4 4.91E–4 3.99E–4 2.27E–4 343.18 2.10E–4823 250 8.58E–4 5.24E–4 2.98E–4 1.79E–4 1.05E–4 847.41 8.05E–5823 240 7.02E–4 5.78E–4 4.73E–4 2.06E–4 1.04E–4 738.18 8.33E–5823 230 4.40E–4 3.02E–4 1.25E–4 5.30E–5 3.26E–5 2583.93 2.63E–5863 250 4.15E–2 7.24E–3 4.87E–3 2.98E–3 2.02E–3 39.88 1.77E–3863 240 1.00E–2 8.26E–3 6.59E–3 3.83E–3 2.55E–3 36.95 1.95E–3863 220 4.66E–3 4.16E–3 3.59E–3 1.56E–3 9.33E–4 127.64 7.12E–4863 200 1.19E–3 9.91E–4 4.93E–4 3.27E–4 2.17E–4 300.15 1.90E–4863 180 6.70E–4 6.22E–4 3.88E–4 1.53E–4 9.83E–5 573.82 9.06E–5863 165 7.20E–4 6.68E–4 5.78E–4 1.89E–4 7.40E–5 1433.8 4.10E-5

Creep rates at p strain were measured from the data points making up the experimental creep curves using a second order version of a lagrange interpolatingpolynomial.

T AB L E I B Results making up the longer-term data set

Creep rate (h−1) at p strain

Stress (MPa) 0.05% 0.1% 0.2% 0.5% 1% Failure time (h)Ruptureelongation (%)

Min. creep rate(h−1)

215 – – – – – 1359 27.2 –185 – – – – – 2956 21.7 –185 – – – – – 3660 19.6 –170 – – – – – 8623 22.0 –170 – 9.2E–5 2.0E–5 4.6E–6 1.7E–6 13559 15.4 2.5E–06154 – – – – – 24328 15.5 –139 4.4E–5 7.5E–6 4.0E–6 2.01E–6 1.2E–6 30558 15.1 1.1E–06139 – 8.2E–6 4.0E–6 7.9E–7 – – – –139 – 1.1E–5 4.5E–6 9.8E–7 – – – –108 4.3E–6 9.0E–7 45E–7 2.5E–7 2.3E–7 – – 2.1E–0777 1.5E–6 2.2E–7 1.0E–7 5.6E–8 – – – –77 1.6E–6 1.8E–7 7.7E–8 – – – – 4.0E–08

– No observation made. Creep rates at p strain were measured from the strain-time measurements made at p strain using a second order version of a lagrangeinterpolating polynomial.

Evans [14] as to whether the parameters of the Monkman-Grant relation are constant over all temperatures, Evans[15] has shown that these parameters are constant over avery wide range of stresses and at all temperatures below873 K (this assertion is limited to 2.25 CrMo material andwork on long term data for other materials would be abeneficial area for future research).

3.2. The relationship between creep rateswithin the 4-� projection technique

The above 4-� projection technique implies an approx-imate linear dependence in a double logarithmic coor-dinate system between creep rates measured at any lowstrain and the minimum creep rate. Given the nature of

T AB L E I C Longer-term predictions made using the 4-� projectiontechnique at 823 K

Stress (MPa)Predicted Failuretime (h)

Predicted Minimumcreep rate (h−1)

215 3,126 1.9E–5185 10,599 5.1E–6170 19,505 2.6E–6154 35,879 1.4E–6139 65,974 7.2E–7108 222,864 1.9E–777 752,147 4.2E–8

Equation 1 above, this can not be shown algebraically ina closed form expression. However, the βk,l values shownin Table II were used in conjunction with Equation 1b to

3909

T A B L E I I The β parameters of Equation 1b use to simulate �i,k valuesin the 4-� projection technique

βk ,0 βk ,1 βk ,2 βk ,3

k = 1 0.25058 −0.023321 −0.003906 2.34E-05k = 2 −95.97042 0.062727 0.086519 −1.89E-05k = 3 −1.855094 −0.039266 −0.005962 5.53E-05k = 4 −77.03491 0.013713 0.065145 3.12E-05

calculate �i,k values over a very wide range of stressesand temperatures. (These βk,l values are actually the es-timates obtained from the short-term data base describedin Section 2 above). Stresses ranged from 500 down to50 MPa and temperatures from 923 down to 723 K. These�i,k values were then used to calculate minimum creeprates and creep rates at various strains (through the differ-entiation of Equation 1a).

It can be seen from Fig. 1 that on a double logarithmiccoordinate system there is a very good linear relation-ship existing between the minimum creep rate and thecreep rate at p strain within the 4-� projection technique.This relationship does however change with the strainchosen—with the intercept term increasing with increas-ing strain.

3.3. The generalised Monkman-Grant relationFig. 1 suggests a simple approach to predicting minimumcreep rates at close to operating conditions. There is no

need to measure complete creep curves, or from them thetheta values at various accelerated test conditions. Nor isthere a need to extrapolate these theta values. Instead, Nspecimens are tested under accelerated conditions untilfailure. For each specimen, the minimum creep rate ismeasured together with the creep rates at various lowstrains (typically 0.05% through to 1%) and the times tofailure. From this data the following relationship is thenestimated using linear least squares

ln(εi,m) = δ0 + δ1 ln(εi,p) (3a)

where εi,pis the creep rate at p creep strain under accel-erated test condition i. To predict minimum creep ratesaround operating conditions (test condition j), M speci-mens are tested under these conditions until p strain hasbeen reached. These M tests are then discontinued. Themeasured creep rates at p strain, εj,p, are then inserted intoEquation 3a to predict the minimum creep rate

ln(εj,m) = δ0 + δ1 ln(εj,p) (3b)

The time to failure around operating conditions can in turnbe predicted using a generalised Monkman-Grant relationwhich is obtained by substituting Eqs. 3b into Equation 2

ln(tj,f ) = φ0 + φ1 ln(εj,m) (3c)

(εm) = 0.6506(εp)1.0044

R2 = 99.51%

1.0E-121.0E-111.0E-101.0E-091.0E-081.0E-071.0E-061.0E-051.0E-041.0E-031.0E-021.0E-011.0E+001.0E+011.0E+02

1.0E-12 1.0E-10 1.0E-08 1.0E-06 1.0E-04 1.0E-02 1.0E+00 1.0E+02

Creep rate at p% strain (s-1)

Min

imum

cre

ep r

ate

(s-1

)

Creep rates at 1.0% strain

εm = 0.4203(εp)1.0051

R2 = 99.43%

1.0E-121.0E-111.0E-101.0E-091.0E-081.0E-071.0E-061.0E-051.0E-041.0E-031.0E-021.0E-011.0E+001.0E+011.0E+02

1.0E-13 1.0E-11 1.0E-09 1.0E-07 1.0E-05 1.0E-03 1.0E-01 1.0E+01 1.0E+03

Creep rate at p% strain (s-1)

Min

imum

cre

ep r

ate

(s-1

)

Creep rates at 0.1% strain

(εm) = 0.5215(εp)1.0056

R2 = 99.51%

1.0E-121.0E-111.0E-101.0E-091.0E-081.0E-071.0E-061.0E-051.0E-041.0E-031.0E-021.0E-011.0E+001.0E+011.0E+02

1.0E-13 1.0E-11 1.0E-09 1.0E-07 1.0E-05 1.0E-03 1.0E-01 1.0E+01 1.0E+03

Creep rate at p% strain (s-1)

Min

imum

cre

ep r

ate

(s-1

)

Creep rates at 0.5% strain

(εm) = 0.4421(εp)1.0053

R2 = 99.46%

1.0E-13 1.0E-11 1.0E-09 1.0E-07 1.0E-05 1.0E-03 1.0E-01 1.0E+01 1.0E+03

Creep rate at p% strain (s-1)

Min

imum

cre

ep r

ate

(s-1

)

Creep rates at 0.2% strain

Figure 1 The relationship between minimum creep rate and creep rate at p strain implied by the 4-� projection technique.

3910

where φ0 = λ0+λ1δ0 and φ1 = λ1δ1. In all cases thevalues for λ and δ are estimated only from the acceleratedor short-term data set.

The standard Monkman-Grant relation has the advan-tage of being easy to estimate and once the minimumcreep rate is known, the life of the material can be pre-dicted from it using Equation 2. This is attractive becausespecimens can be put on test at operating conditions untilthe minimum creep rate is recorded and then removed. Be-cause this typically occurs well before the materials life, alife prediction can be made well in advance of failure. Thedisadvantage of using the standard Monkman-Grant re-lation to predict safe life is that at operating conditions, itcan still take tens of thousands of hours to reach the mini-mum creep rate and tests of this length are often not viablefrom a practical or economic perspective. The gener-alised Monkman-Grant relation described in Equation 3covercomes this limitation because creep rates at very lowstrains are observed well before the minimum creep rate.

4. Predictive capabilityTo assess the predictive accuracy of the creep propertyprediction models described above, these models are firstestimated using the results from the N specimens makingup the short-term data set. The models are then used topredict the properties of those M specimens tested in thelonger-term data set. One simple measure of predictiveaccuracy is the mean squared prediction error (MSE) orthe mean absolute prediction error (MAE). Often the MSEis square rooted to be in the same units as Yj

M SE = 1

M

M∑

j=1

[Y j − Y j

]2(4a)

M AE = 1

M

M∑

j=1

[∣∣Y j − Y j

∣∣] (4b)

where Yj is the predicted creep property for the specimentested at the jth longer-term test condition and Yj is theactual creep property for this specimen (squares or abso-lute errors are used so that over and underestimates arenot offsetting in the averaging procedure). However, boththe MSE and the MAE lack any sense of scale and thiscan be overcome by expressing the prediction error as apercentage of the actual value

M S P E = 100

M

M∑

j=1

[(Y j − Y j )

Y j

]2

(4c)

M AP E = 100

M

M∑

j=1

[∣∣∣∣∣Y j − Y j

Y j

∣∣∣∣∣

](4d)

The MSE is a useful way of assessing the predictive accu-racy of a creep model because this error, following Theil’s

analysis [16 ], can be decomposed into a number of dif-ferent components

M SE = 1

M

M∑

j=1

e2j = 1

M

M∑

j=1

[(e j − e) + e

]2

and upon expanding the brackets

M SE =∑M

j=1 (e j − e)2

M+e2+ 2ei

∑Mj=1 (e j − e)

M(5a)

where ej = Yj − Yj is the prediction error associated withthe jth test condition in the longer-term data set and e isthe average prediction error calculated from the M longer-term data points. The first expression in Equation 5a is thesample variance of the prediction error (biased in smallsamples), S2

e , and for any sample the (e − e) term alwayssums to zero so

M SE = e2 + S2e (5b)

A good model will predict with an average error close tozero and with only small over/under predictions aroundthis average, i.e. small variation in the prediction error. Aplot of actual versus predicted creep property values canbe used to further decompose this MSE. On such a plot,all the data points should fall on a one to one line if thecreep prediction model is a perfect predictor. That is α =0, β = 1 and S2

ε = 0 in

Y j = α + βY j + ε j (6)

where εj is the extent to which the jth creep propertyprediction differs from α + βYj, and S2

ε is the variance insuch disturbances. Rearranging Equation 6 above for theprediction error gives

(Y j − Y j ) = e j = α + (β − 1)Y j + εi (7)

Assuming that Yi and εi are independent of each other itfollows from Equations 7 and 5b that

MSE = e2 + {(β − 1)2S2

Y

} + S2ε (8a)

where S2Y

is the variance of the predictions. Thus

1 = e2

M SE+

{(β − 1)2S2

Y

}

M SE+ S2

ε

M SE= UM + UR + UD (8b)

Equation 8b shows that a proportion of the MSE is dueto the average of the models predictions differing fromthe average of the actual values UM. Another part is dueto the slope of the best fit line on the actual v predictionplot differing from 1, UR. Both UM and UR thereforerepresent systematic errors and large values for these twoterms suggest that the creep model is incomplete in some

3911

way. For example, it may suggest that some explanatoryvariables are missing from the model, or that the modelsfunctional relationship between the creep property andtest conditions is incorrect. A final part of the MSE is dueto the data points on the actual v prediction plot not alllying on the best fit line, UD. When they all lie on thebest fit line S2

ε = 0. As the εi are random in nature, UD

represents random prediction errors that can’t be reduced.Ideally, a creep property model should have a very smallMSE with UM = UR

∼= 0 and 1 ∼= UD.

5. Creep property predictions using thetraditional and simplified 4-� models

5.1. Predicting minimum creep ratesFig. 2a shows the actual relationships existing betweencreep rates at various low strains and the minimumcreep rate both in the short and longer-term data sets.At each chosen strain there is a clear linear correlationbetween the logarithmic creep rate at that strain and thelogarithmic minimum creep rate within the short-termdata set. For example, the logarithmic creep rate at0.1% strain can explain 93.01% of the variation in thelogarithmic minimum creep rate in the short-term dataset. This rises to 99.3% when using the creep rate at1% strain. At all strains the value for δ1 in Equation 3aappears to fluctuate randomly around a value of unity.However, δ0 appears to increase with increasing strainand these two results are consistent with that to beexpected from the 4-� projection technique.

Fig. 2a also shows that at all strains, a reasonable pre-diction of the minimum creep rate in the longer-term dataset can be made. The accuracy of these predictions arequantified in Table III where the MAPE and the MSE to-gether with its decomposition (given by Equation 8b) areshown. The 4-� projection technique produced a MAPEof just 47.37%. Further, the majority of the errors madein predicting the minimum creep rate in this way werenot random in nature. These systematic errors made inpredicting the minimum creep rate amounted to 92.51%,with 30.57% of the MSE attributable to the average ofthe models predictions differing from the average of theactual values and 61.94% of the MSE attributable to theslope of the best fit line on the actual v prediction plotdiffering from unity. Only 7.49% of the prediction errorswere random in nature.

In contrast to this, the best of the generalised Monkman-Grant relations (based on the MAPE) used the creep ratesat 0.5% and 1.0% strains. For example, using creep ratesat 0.5% strain the majority of the errors made in predict-ing the minimum creep rate are now random in nature(52.8%). The systematic errors made in predicting theminimum creep rate amounted to 47.2%, with 1.07% ofthe MSE attributable to the average of the models predic-tions differing from the average of the actual values and46.13% of the MSE attributable to the slope of the bestfit line on the actual v prediction plot differing from 1.Indeed both these models perform much better than the4-� projection technique.

εm = 0.2454(ε0.2)0.9863

R2 = 0.9365

1.0E-08

1.0E-07

1.0E-06

1.0E-05

1.0E-04

1.0E-03

1.0E-02

1.0E-08 1.0E-07 1.0E-06 1.0E-05 1.0E-04 1.0E-03 1.0E-02 1.0E-01

Creep rate at 0.2% strain, (h-1),ε0.2

Min

imum

cre

ep r

ate

(h -1

), ε

m

Short term data

Longer term data

Longer-term predictions

εm = 0.4667(ε0.5)0.9721

R2 = 0.963

1.0E-08

1.0E-07

1.0E-06

1.0E-05

1.0E-04

1.0E-03

1.0E-02

1.0E-08 1.0E-07 1.0E-06 1.0E-05 1.0E-04 1.0E-03 1.0E-02

Creep rate at 0.5% strain,(h-1), ε0.5

Min

imum

cre

ep r

ate

(h -1

), ε

m

Short-term data

Longer-term data

Longer-term predictionsεm = 0.9731(ε1)

1.0139

R2 = 0.993

1.0E-08

1.0E-07

1.0E-06

1.0E-05

1.0E-04

1.0E-03

1.0E-02

1.0E-07 1.0E-06 1.0E-05 1.0E-04 1.0E-03 1.0E-02

Ctrain rate at 1.00% strain,(h-1), ε1.00

Min

imum

cre

ep r

ate

(h -1

), ε

m

Short term data

Longer-term data

Extrapolations

εm = 0.241(ε0.1)1.0466

R2 = 0.9301

1.0E-08

1.0E-07

1.0E-06

1.0E-05

1.0E-04

1.0E-03

1.0E-02

1.0E-07 1.0E-06 1.0E-05 1.0E-04 1.0E-03 1.0E-02 1.0E-01

Creep rate at 0.1% strain, (h-1), ε0.1

Min

imum

cre

ep r

ate,

(h

-1),

εm

Short-term data

Longer-term data

Longer-term predictions

(a)

Figure 2 (a) The observed experimental relationship between minimum creep rate and creep rate at p strain. (b) The observed experimental relationshipbetween failure time and creep rate at p strain.

3912

tf = 0.0977(ε1.0)-0.9515

R2 = 0.95221

10

100

1000

10000

100000

1000000

1.0E-07 1.0E-06 1.0E-05 1.0E-04 1.0E-03 1.0E-02

Creep rate at 1.0% strain, (h-1), ε1.0

Tim

e to

fai

lure

(h)

, tf

Short-term data

Longer-term data

Longer-term predictions

tf = 0.3323(ε0.1)-0.9951

R2 = 0.915210

100

1000

10000

100000

1000000

10000000

0.0000001 0.000001 0.00001 0.0001 0.001 0.01 0.1

Creep rate at 0.1% strain, (h-1),ε0.1

Tim

e to

fai

lure

(h)

, tf

Short-term data

Longer-term data

Longer-term predictions

tf = 0.3547(ε0.2)-0.9261

R2 = 0.89891

10

100

1000

10000

100000

1000000

10000000

1E-08 1E-07 0.000001 0.00001 0.0001 0.001 0.01 0.1

Creep rate at 0.2% strain, (h-1),ε0.2

Tim

e to

fai

lure

, (h)

, tf

Short-term data

Longer-term data

Longer-term predictions

tf= 0.2087(ε0.5)-0.9035

R2 = 0.90551

10

100

1000

10000

100000

1000000

0.00000001 0.0000001 0.000001 0.00001 0.0001 0.001 0.01

Creep rate at 0.5% strain, (h-1),ε0.5

Tim

e to

fai

lure

(h)

, tf

Short-term data

Longer-term data

Longer-term predictions

(b)

Figure 2 Continued.

Even when creep rates at lower strains are used, themodels perform reasonable well with acceptable MAPE,although the majority of the errors made in predicting theminimum creep rate are then systematic in nature. Thismay reflect the larger errors made in measuring creep ratesvery early on in a creep curves evolution. What stands outfrom this is that the extra complexity involved with usingthe 4-� projection technique as compared to the gener-alised Monkman-Grant relations does not reflect itself in aproportionate improvement in predictive accuracy. How-ever, there remains the question of which level of strainto measure the creep rate. A future paper will addressthis issue further by assessing whether a combination ofstrains is best.

5.2. Predicting times to failureFig. 2b shows the actual relationship existing betweenthe minimum creep rates at various low strains and time

to failure both in the short and longer-term data sets.At each chosen strain there is a clear linear correlationbetween the logarithm of the creep rate at that strainand the logarithmic time to failure within the short-termdata set. For example, the logarithmic creep rate at 0.1%strain can explain 91.52% of the variation in the loga-rithm of the time to failure in the short-term data set.This rises to 95.2% when using the creep rate at 1%strain. It can also be seen that the generalised Monkman-Grant relations shown Fig. 2b extrapolate well to thelonger-term data even at low strains. This is because theR2 values associated with the lowest strains do not ap-pear to be very much lower than that associated with1% strain or indeed the minimum creep rate over theshort-term data. (The R2 associated with the Monkman-Grant relation is 97%). At all strains the value for ϕ1 inEquation 3c appears to fluctuate just below a value ofunity. However, ϕ0 appears to decrease with increasingstrain.

T AB L E I I I The MAPE, MSE and MSE decomposition for predictions of the minimum creep rate

PredictiveGeneralised Monkman-Grant models using creep rates at:

statistics 0.1% strain 0.2% strain 0.5% strain 1% strain 4-�

MAPE 94.25% 36.76% 25.40% 22.90% 47.37%MSE 2.04E–11 1.49E–12 1.36E–13 4.30E–13 3.36E–13UM 15.12% 16.48% 1.07% 41.79% 30.57%UR 84.14% 79.06% 46.13% 36.75% 61.94%UD 0.74% 4.46% 52.80% 21.46% 7.49%

3913

100

1000

10 100 1000 10000 100000 1000000

Time to Failure, (h), tf

Str

ess,

(M

Pa)

τ

Actual short-term dataActual longer-term data4-theta predictionsGeneralised Monkman -Grant predictions (p = 0.1%)Generalised Monkman -Grant predictions (p = 0.2%)

Figure 3 Predicted ln(τ )/ln(tf ) plots for constant stress conditions, compared with the measured tf values obtained from short-term constant-st 823 K.

Fig. 3 gives a slightly different perspective on the shortand longer-term predictions shown in Fig. 2b. In Fig. 3 theactual times to failure, predicted times to failure associ-ated with the generalised Monkman-Grant relation (withcreep rates measured at 0.1 and 0.2% strain) and predictedtimes to failure given by the 4-� projection technique at823 K are plotted against various stresses. All these proce-dures produce good predictions of the short term data, butthe generalised Monkman-Grant relation does not overes-timate the longer-term data to the same extent as the 4-�projection technique. (Note how only the 4-� projectiontechnique produces predictions that are a smooth functionof stress).

Table IV further quantifies the accuracy of the projec-tions shown in Figures 2b and 3 using the MAPE and theMSE associated with the predicted times to failure. Alsoshown for each of these predictions is a decompositionof the MSE using Equation 8b above. The 4-� projectiontechnique produced a MAPE of just over 100%. Further,the majority of the errors made in predicting the times

to failure were systematic in nature. For example, around81% of the MSE is attributable to the average of the modelspredictions differing from the average of the actual values.Around 14% of the MSE was random in composition. Incontrast, the best of the generalised Monkman-Grant re-lations used the creep rate measured at 0.2%. This modelproduced a MAPE of around 18%. However, the majorityof the errors made in predicting the times to failure wereagain systematic in nature. Around 77% of the MSE isattributable to the average of the models predictions dif-fering from the average of the actual values and around22% of the MSE was random in composition.

The predictive capability of the other generalisedMonkman-Grant relations models were not so good as theone above. This again raises the question of which strainto use. It may be possible to combine the predictions fromall the generalised Monkman-Grant relations models intoa single improved prediction of time to failure. This issueon combinations of forecasts will be addressed in a futurepaper.

T AB L E I V The MAPE, MSE and MSE decomposition for predictions of the time to failure

PredictiveGeneralised Monkman-Grant models using creep rates at:

statistics 0.1% strain 0.2% strain 0.5% strain 1% strain 4-�

MAPE 40.35% 18.39% 66.44% 103.37% 103.54%MSE 5.77E+7 7.75E+8 2.16E+10 1.5E+9 2.76E+9UM 0.28% 76.91% 72.14% 97.88% 81.24%UR 83.67% 1.38% 17.53% 1.64% 4.73%UD 16.06% 21.71% 10.33% 0.48% 14.02%

3914

The poorer performance (based on the MAPE) of the 4-� projection technique relative to most of the generalisedMonkman-Grant relations probably reflect the poorer per-formance of the 4-� projection technique in predictingminimum creep rates. This in turn may be the result ofobtaining a good fit to the tertiary part of the creep curvein the 4-� projection technique.

Finally, it can be noted from Tables III and IV thatthe MSE and the MAPE give slightly different rankingsof all the different approaches described above. Whenranking techniques in this way it is always best to use theMAPE because, unlike the MSE, it scales the predictionerror relative to the actual value. Further, the MSE can bedistorted by a few large prediction errors as a result ofthe squaring procedure—a problem avoided through theuse of absolute values. The MSE is useful only because itcan be easily decomposed into a systematic and randomcomponent (in a way that the MAPE can’t). As an absolutemeasure of predictive accuracy it can be misleading.

6. ConclusionIt has been demonstrated, using simple simulations, that alinear dependence in a double logarithmic coordinate sys-tem exists between creep rates measured at any low strainand the minimum creep rate if creep obeys the equationsmaking up the 4-� projection technique. This provides forthe possibility of modelling creep properties using gen-eralised Monkman-Grant relations—that differ only bythe low strain chosen to measure the creep rate which isused to predict the minimum creep rate. Short-term exper-imental data confirms that such a relationship does indeedappear to exist. Further, this relationship also holds intothe longer-term data so that the generalised Monkman-Grant relation produces good predictions of the minimumcreep rates observed in the longer-term data. Indeed, allbut the generalised Monkman-Grant relation using 0.1%strain had a lower MAPE compared to the 4-�projectiontechnique. The generalised Monkman-Grant relation us-ing 0.5 and 1% strains had larger random components ofthe MSE compared to the 4-�projection technique (and avery similar random component at 0.2%).

When considering the accuracy with which times tofailure were predicted all of the generalised Monkman-Grant relations produced lower MAPE compared to the

4-� projection technique. However, only when creeprates were measured at 0.2% strain, did the generalisedMonkman-Grant relation produce prediction errors thathad a significantly higher random component comparedto the traditional 4-� projection technique.

The predictive capability of some generalisedMonkman-Grant relations were much better than othersand so the question of at which strain should creep ratesbe measured appears again to be critical. It may be pos-sible to combine the predictions from all the generalisedMonkman-Grant relations into a single improved predic-tion of time to failure. This issue on combinations offorecasts will be addressed in a future paper.

References1. M. E VA N S , J. Mater Sci. 39 (2004) 2053.2. R . W. E VA N S , Mat. Sci. Technol. 5 (1989) 699.3. Idem. ibid. 16 (2000) 6.4. R . W. E VA N S and P. J . S C H A R N I N G , Mat. Sci. Technol., 17

(2001) 487.5. L . M. K AC H A N OV , “The Theory of Creep” (National Lending

Library, Boston Spa, UK, 1967).6. Y. N . R A B OT N OV , “Creep Problems in Structural Members”

(North Holland, Amsterdam, 1969).7. A . M. OT H M A N and D. R . H AY H U R S T , Int. J. Mech. Sci. 32(1)

(1990) 35.8. M. P R AG E R , The Omega Method—An Engineering Approach to Life

Assessment. Journal of Pressure Vessels Technology 122 (2000) 273.9. R . W. E VA N S and B. W I L S H I R E , “Creep of Metals and Alloys”

(The Institute of Materials, London, 1985).10. R . W. E VA N S , M. R . W I L L I S , B . W I L S H I R E , S .

H O L D S W O RT H , B . S E N I O R , A . F L E M I N G , M. S P I N D L E R

and J . A . W I L L I A M S , in Proceedings of the 5th InternationalConference on “Creep and Fracture of Materials and Structures”,Swansea, 1993, edited by B. Wilshire and R.W. Evans (The Instituteof Materials, London, 1993) p. 633.

11. M. E VA N S , J. Mater Sci. 35 (2000) 2937.12. F. C . M O N K M A N and N. J . G R A N T , edited by N. J. Grant and

A. W. Mullendore (MIT Press, Boston, 1963) vol. 56.13. F. D O B E S and K. M I L I C K A , Met. Sci. 10 (1976) 382.14. M. E VA N S , Mater Sci. Technol. 15 (1999) 91.15. M. E VA N S , in Proceeding of the International Conference on “Creep

and Fracture in High Temperature Components—Design and LifeAssessment Issues”, London 2005, organized by the European CreepCollaborative Committee.

16. H . T H E I L , “Applied Economic Forecasting” (Rand McNally &Company, 1966).

Received 6 Juneand accepted 8 June 2005

3915